Hydrogen sensors based on electrophoretically deposited Pd nanoparticles onto InP
© Grym et al; licensee Springer. 2011
Received: 12 November 2010
Accepted: 20 May 2011
Published: 20 May 2011
Electrophoretic deposition of palladium nanoparticles prepared by the reverse micelle technique onto InP substrates is addressed. We demonstrate that the substrate pre-deposition treatment and the deposition conditions can extensively influence the morphology of the deposited palladium nanoparticle films. Schottky diodes based on these films show notably high values of the barrier height and of the rectification ratio giving evidence of a small degree of the Fermi level pinning. Moreover, electrical characteristics of these diodes are exceptionally sensitive to the exposure to gas mixtures with small hydrogen content.
Metal nanoparticles (MNPs) form a bridge between bulk materials and atomic or molecular structures. Bulk metals show constant size-independent physical properties, while the properties of MNPs are driven by their size, shape, and inter-particle distance. Surface properties are crucial because the number of surface atoms becomes significant as the MNP reaches the nanoscale limit . III-V semiconductors have established their position in electronic devices thanks to their unique properties. As compared to silicon, they offer higher operating speeds, lower power consumption, or higher light emission efficiency. However, to fully exploit their properties, there is one key point remaining to be solved. III-V semiconductor structures suffer from a high density of surface/interface states causing so called Fermi level pinning (FLP) . The mechanism responsible for the FLP at the metal-semiconductor interface has been a subject of a long-term discussion. We consider the disorder-induced gap state model stating that large energy deposition processes cause large disorder at the interface and thus a strong FLP . The FLP leads to low Schottky barrier heights (SBH) on n-type III-Vs, which are metal independent when prepared by standard evaporation techniques . Substantial improvements were reached by (i) incorporation of a thin native oxide , (ii) low-energy electrochemical deposition [6, 7], and (iii) electroless plating .
In this article, we report on the preparation of Schottky barriers on InP substrates with increased SBHs by the electrophoretic deposition of palladium nanoparticles (NPs). We also demonstrate their application in hydrogen sensors. Regarding the group VIII transition metals, palladium and platinum are the two most preferred catalytic metals that have an outstanding capability of absorbing hydrogen . Hydrogen molecules are adsorbed at the metal surface and partly dissociated into atoms. These atoms can diffuse through the metal to the interface with a semiconductor changing the SBH and accordingly the electrical properties of the structure. The hydrogen detection sensitivity and the Schottky barrier quality can be improved by reducing the metal grain size [10–12].
Pd NPs dispersed in isooctane solution were prepared by the reverse micelle technique . Two reverse micelle solutions with identical molar ratio of water to AOT (sodium di-2-ethylhexylsulfosuccinate) were prepared. The first one was an aqueous solution of Pd(NH3)4Cl2, the second was an aqueous solution of hydrazine. Equal volumes of these solutions were mixed leading to the reduction of Pd(NH3)4Cl2 by hydrazine within the reverse micelles. As a result, Pd NPs with the diameters of 7 to 10 nm embedded in reverse micelles of AOT dispersed in isooctane were obtained.
The electrophoretic deposition from the colloid solution took place in a cell with two parallel electrodes. The upper electrode was made from high-purity graphite, the lower electrode was formed by an epi-ready InP substrate of n-type conductivity with the background concentration of about 6 × 1015 cm-3. The substrates were cleaved from epi-ready wafers and all handling and depositions were conducted in a clean room facility. A back side ohmic contact to the InP substrate was formed by either rubbing liquid gallium with a tin rod or by vacuum evaporation of AuGeNi alloy. The distance between the electrodes was maintained at 1.5 mm. Pulsed DC voltage with a duty cycle of 50% and frequency of 10 kHz was applied for a selected period of time to deposit a Pd nanolayer. The pulsed voltage regime favors the deposition of individual nanoparticles over the deposition of nanoparticle clusters [14, 15]. The deposition process was described in detail in . Some of the substrates with deposited nanolayers were further annealed at 400°C in a vacuum of 10-5 torr.
Layers of NPs were observed in JEOL JSM 7500F scanning electron microscope and by atomic force microscopy (AFM). Selected layers were contacted by the spots of a graphite colloid paint. These structures were further characterized by the measurement of current-voltage characteristics and their detection toward hydrogen was tested in a cell with a through-flow gas system.
Results and discussion
We discuss the influence of (i) the final substrate surface treatment, (ii) the properties of the deposited colloid solution, (iii) the elecrophoretic deposition conditions (time, electrode polarity, applied voltage), and (iv) the post-deposition treatment of the layers (annealing at elevated temperatures) on the morphology of the deposited layers, their electrical properties, and their sensitivity toward hydrogen.
Second, different surface treatments of InP substrates were performed. Conventional procedures for cleaning the substrates of III-V semiconductors consist in refluxing the substrate in a sequence of organic solvents such as trichloroethylene, acetone, methanol, and isopropyl alcohol to remove the contamination from heavy hydrocarbons, particles and heavy-atom contaminants . The surface of epi-ready InP was (i) multiply rinsed in isooctane, (ii) treated in boiling methanol for 3 min, or (iii) treated in boiling isopropyl alcohol for 3 min. Different surface treatments significantly influenced the morphology of Pd nanolayers. While on the substrates treated in isooctane and isopropyl alcohol large clusters of Pd NPs were deposited, individual Pd NPs were observed on the substrates treated in methanol, which is in accordance with the conclusions of das Neves and de Paoli  that a single rinse in methanol can substitute a multiple rinse in different organic solvents, while a single rinse in isopropyl alcohol is insufficient for the preparation of a clean substrate surface.
Third, deposition times were varied to reach a different surface coverage. As expected, higher deposition times resulted in higher surface coverage (Figure 1c, d, e, f). Even at relatively long deposition times, the surface was not covered completely (Figure 1e). A full coverage was achieved by a multiple deposition (Figure 1f). This indicates that the colloid solution gradually depletes of Pd NPs. Moreover, at high deposition times (without changing the colloid solution), not only the Pd NPs are deposited, but also increased amounts of the surfactant (AOT) are observed on the surface by SEM.
Finally, some of the layers were annealed for 1 h at 400°C. This temperature was a compromise to remove AOT and not to cause damage to the InP substrate, which starts to decompose above 360°C. Luwang et al. investigated thermal properties of SnO2/AOT NPs in argon and air. They assigned exotermic peaks at 340°C to the decomposition of AOT . Park et al. studied CdS/AOT and CdS/ZnS/AOT NPs in nitrogen and air and observed weight reduction due to the AOT removal from 220 to 380°C. The Fourier transform infrared spectroscopy showed that bands related to AOT were smaller on the samples subjected to 2-h treatment at 570°C compared to untreated samples; however, did not disappear completely . Concerning the observation in SEM, after annealing, it was easier to observe individual Pd NPs, their round shape was truly visible, and no charging effects were experienced implying that remnants of the surfactant were partially removed. Also, adhesion of the layers was greatly enhanced. Non-annealed layers are susceptible to surface damage; improper handling leads to their partial removal. Besides, AFM observation is intricate as the AFM tip pushes the NPs toward the borders of the scanned area.
Electrical properties and hydrogen detection
Two sets of samples were contacted by the graphite colloid paint to measure current-voltage (I-V) characteristics of the InP/Pd NPs/graphite structures and to characterize its capability of detecting hydrogen. Graphite can be deposited at room temperature and causes minimum disturbance to the semiconductor surface; it was reported to form good Schottky contacts on different semiconductors [22, 23].
Summary of the deposition conditions and electrical characteristics of the samples prepared on methanol-treated substrates
R at 1.5 V
ϕ b (eV)
S at 0.1%H2
Preparation of Pd NPs by the reverse micelle technique and their electrophoretic deposition onto InP substrates were discussed. We were able to vary the surface morphology of the films formed by Pd NPs from several individual NPs on the surface to its full coverage. Variety of morphologies was achieved by changing the substrate pre-deposition treatment and the deposition conditions. Schottky diodes based on these films showed notably high values of the barrier height up to 0.95 eV and of the rectification ratio up to 4.8 × 107 giving evidence of a small degree of the Fermi level pinning. Moreover, electrical characteristics of these diodes were exceptionally sensitive to the exposure to gas mixtures with small hydrogen content. An outstanding value of the sensing response of 4.8 × 105 was achieved for the 0.1% H2/N2 mixture pointing to the bright prospects of these structures in extremely sensitive hydrogen sensors.
atomic force microscopy
Fermi level pinning
Schottky barrier height.
We thank Dr. K. Zdansky for rewarding comments. The study was supported by the projects 102/09/1037 of the Czech Science Foundation and grant KJB200670901 of the ASCR.
- Hossam H: Chemical sensors based on molecularly modified metallic nanoparticles. J Phys D 2007, 40(23):7173–7186. 10.1088/0022-3727/40/23/S01View Article
- Hasegawa H, Akazawa M: Interface models and processing technologies for surface passivation and interface control in III-V semiconductor nanoelectronics. Appl Surf Sci 2008, 254(24):8005–8015. 10.1016/j.apsusc.2008.03.051View Article
- Hasegawa H, Ohno H: Unified disorder induced gap state model for insulator-semiconductor and metal-semiconductor interfaces. J Vac Sci Technol B 1986, 4(4):1130–1138. 10.1116/1.583556View Article
- Hokelek E, Robinson GY: A study of Schottky contacts on indium phosphide. J Appl Phys 1983, 54(9):5199–5205. 10.1063/1.332745View Article
- Wada O, Majerfeld A, Robson PN: InP Schottky contacts with increased barrier height. Solid-State Electron 1982, 25(5):381–387. 10.1016/0038-1101(82)90123-XView Article
- Hasegawa H: Inteface-controlled Schottky barriers on InP and related materials. Solid-State Electron 1997, 41(10):1441–1450. 10.1016/S0038-1101(97)00087-7View Article
- Hasegawa H: Fermi level pinning and Schottky barrier height control at metal-semiconductor interfaces of InP and related materials. Jpn J Appl Phys 1999, 38(2B):1098–1102.View Article
- Chen HI, Chou YI, Chu CY: A novel high-sensitive Pd/InP hydrogen sensor fabricated by electroless plating. Sens Actuators B 2002, 85(1–2):10–18. 10.1016/S0925-4005(02)00044-8View Article
- Carturan G, Cocco G, Facchin G, Navazio G: Phenylacetylene hydrogenation with Pd, Pt and Pd-Pt Alloy catalysts dispersed on amorphous supports - effect of Pt/Pd ratio on catalytic activity and selectivity. J Mol Catal 1984, 26(3):375–384. 10.1016/0304-5102(84)85111-1View Article
- Sato T, Uno S, Hashizume T, Hasegawa H: Large Schottky barrier heights on indium phosphide-based materials realized by in-situ electrochemical process. Jpn J Appl Phys 1997, 36(3B):1811–1817.View Article
- Chou YI, Chen CM, Liu WC, Chen HI: A new Pd-InP Schottky hydrogen sensor fabricated by electrophoretic deposition with Pd nanoparticles. IEEE Electron Device Lett 2005, 26(2):62–65.View Article
- Kimura T, Hasegawa H, Sato T, Hashizume T: Sensing mechanism of InP hydrogen sensors using Pt Schottky diodes formed by electrochemical process. Jpn J Appl Phys 2006, 45(4B):3414–3422. 10.1143/JJAP.45.3414View Article
- Chen D-H, Wang C-C, Huang T-C: Preparation of palladium ultrafine particles in reverse micelles. J Colloid Interface Sci 1999, 210(1):123–129. 10.1006/jcis.1998.5795View Article
- Naim MN, Iijima M, Kamiya H, Lenggoro IW: Electrophoretic packing structure from aqueous nanoparticle suspension in pulse DC charging. Colloids Surf A 2010, 360(1–3):13–19. 10.1016/j.colsurfa.2010.01.057View Article
- Naim MN, Iijima M, Sasaki K, Kuwata M, Kamiya H, Lenggoro IW: Electrical-driven disaggregation of the two-dimensional assembly of colloidal polymer particles under pulse DC charging. Adv Powder Technol 2010, 21(5):534–541. 10.1016/j.apt.2010.02.004View Article
- Zdansky K, Zavadil J, Kacerovsky P, Lorincik J, Vanis J, Kostka F, Cernohorsky O, Fojtik A, Reboun J, Cermak J: Electrophoresis deposition of metal nanoparticles with reverse micelles onto InP. Int J Mater Res 2009, 100(9):1234–1238.View Article
- Sarkar P, De D, Yamashita K, Nicholson PS, Umegaki T: Mimicking nanometer atomic processes on a micrometer scale via electrophoretic deposition. J Am Ceram Soc 2000, 83(6):1399–1401. 10.1111/j.1151-2916.2000.tb01400.xView Article
- Ingrey S: III-V-Surface processing. J Vac Sci Technol A 1992, 10(4):829–836. 10.1116/1.577680View Article
- Das Neves S, De Paoli MA: Monitoring the organic cleaning process of Inp crystals by contact-angle measurement. Semiconductor Sci Technol 1994, 9(9):1719–1721. 10.1088/0268-1242/9/9/023View Article
- Luwang MN, Ningthoujam RS, Singh NS, Tewari R, Srivastava SK, Vatsa RK: Surface chemistry of surfactant AOT-stabilized SnO2 nanoparticles and effect of temperature. J Colloid Interface Sci 2010, 349(1):27–33. 10.1016/j.jcis.2010.05.037View Article
- Park K, Yu H, Chung W, Kim B-J, Kim S: Effect of heat-treatment on CdS and CdS/ZnS nanoparticles. J Mater Sci 2009, 44(16):4315–4320. 10.1007/s10853-009-3641-2View Article
- Tongay S, Schumann T, Hebard AF: Graphite based Schottky diodes formed on Si, GaAs, and 4H-SiC substrates. Appl Phys Lett 2009, 95(22):222103–222103. 10.1063/1.3268788View Article
- Tongay S, Schumann T, Miao X, Appleton BR, Hebard AF: Tuning Schottky diodes at the many-layer-graphene/semiconductor interface by doping. Carbon 2011, 49(6):2033–2038. 10.1016/j.carbon.2011.01.029View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.